# Www.lightsource.ca Introduction to Crystallography Joel Reid, Canadian Light Source, Inc. Canadian Powder Diffraction Workshop 2012.

## Presentation on theme: "Www.lightsource.ca Introduction to Crystallography Joel Reid, Canadian Light Source, Inc. Canadian Powder Diffraction Workshop 2012."— Presentation transcript:

www.lightsource.ca Introduction to Crystallography Joel Reid, Canadian Light Source, Inc. Canadian Powder Diffraction Workshop 2012

www.lightsource.ca Outline Crystal structures, lattices & crystal systems. Elements of point symmetry, point groups. Translation symmetry, space groups, equivalent positions, special positions and site multiplicities. Powder diffraction, reflection positions and intensities.

www.lightsource.ca What is a Crystal Structure? A crystal structure is a pattern of atoms which repeats periodically in three dimensions (3D). The pattern can be as simple as a single atom, or complicated like a large organic molecule or protein. The periodic repetition can be represented using a 3D lattice. The atomic pattern and the lattice generally both exhibit elements of symmetry.

www.lightsource.ca What is Symmetry? An object has symmetry if an operation or movement leaves the object in a position indistinguishable from the original position. Crystals have two types of symmetry we have to consider: Point symmetry (associated with the atomic pattern). Translational symmetry (associated with the crystal lattice).

www.lightsource.ca What is a Lattice? Consider a periodic pattern in 2D. A system of points can be obtained by choosing a random point with respect to the pattern. All other points identical to the original point form a set of lattice points.

www.lightsource.ca Lattice Points and Unit Cells By connecting our lattice points, we divide the area into parallelograms. Each parallelogram represents a unit cell, a basic building block which can be used to replicate the entire structure.

www.lightsource.ca Unit Cell (2D) The size and shape of the unit cell can be described by 2 basis vectors (two edge lengths, a & b, and the angle γ). Any position in the unit cell can be described in terms of the basis vectors with fractional coordinates: Point p → (1, ½) = 1 a + 0.5 b Every lattice point can be generated by integer translations of the basis vectors (t = ua + vb, where u & v are integers).

www.lightsource.ca Choice of Unit Cell The choice of unit cell is not unique. A unit cell with lattice points only at the corners (1 lattice point per cell) is called primitive, while a unit cell with additional lattice points is called centered.

www.lightsource.ca 2D Planar Systems Figure courtesy of Michael Gharghouri.

www.lightsource.ca Unit Cell (3D) The 3D unit cell size and shape can be fully described using 3 basis vectors (three lengths a, b & c and three angles α, β & γ).

www.lightsource.ca 3D Crystal Systems SystemLattice Parameter Restrictions Bravais Lattices Triclinic (Anorthic) a, b, c, α, β, γaP Monoclinica, b, c, 90, β, 90mP, mC Orthorhombica, b, c, 90, 90, 90oP, oC, oI, oF Trigonala, a, a, α, α, α a, a, c, 90, 90, 120 R hP Hexagonala, a, c, 90, 90, 120hP Tetragonala, a, c, 90, 90, 90tP, tI Cubica, a, a, 90, 90, 90 cP, cI, cF Figure courtesy of Michael Gharghouri.

www.lightsource.ca Bravais Lattices Figure adapted from: http://www.seas.upenn.edu/~chem101/sschem/solidstatechem.html

www.lightsource.ca Types of Symmetry The lattice and unit cell basis vectors describe aspects of the translational symmetry of the crystal structure. However, we also have to consider symmetry elements inherent to the atoms and molecules within the unit cell. The symmetry elements of finite molecules are called point symmetry.

www.lightsource.ca What is Point Symmetry? A point symmetry operation always leaves at least one point fixed (an entire line or plane may remain fixed). Rotation axes, mirror planes, centers of symmetry (inversion points) and improper rotation axes are all elements of point symmetry. Collections of point symmetry elements describing finite molecules are called point groups.

www.lightsource.ca Rotation Axes A rotation of 360°/n is referred to with the symbols n (Hermann-Mauguin notation) or C n (Schoenflies notation). Crystals are restricted (in 3D) to 1, 2, 3, 4 & 6 rotation axes. Figures taken from: Sands, D.E., Introduction to Crystallography. (Dover: New York, 1993) 3 or C 3 axis

www.lightsource.ca Mirror Planes A mirror (or reflection) plane is referred to as m (Hermann-Mauguin) or σ (Schoenflies). Figures taken from: Sands, D.E., Introduction to Crystallography. (Dover: New York, 1993)

www.lightsource.ca Center of Symmetry (Inversion) Figure taken from: Sands, D.E., Introduction to Crystallography. (Dover: New York, 1993)

www.lightsource.ca Improper Rotation Axes

www.lightsource.ca Improper Rotation Axes Figure taken from: Sands, D.E., Introduction to Crystallography. (Dover: New York, 1993)

www.lightsource.ca Elements of Point Symmetry ElementHermann-Mauguin Symbols Schoenflies Symbols Rotation Axis1,2,3,4,6C 1, C 2, C 3, C 4, C 6 Mirror Planemσ Identity1E = C 1 Center of Symmetry (Inversion) i Rotary Inversion (or Reflection) Axis S 2, S 1, S 6, S 4, S 3

www.lightsource.ca Point Groups The point group refers to the collection of point symmetry elements possessed by an atomic or molecular pattern. There are 32 point groups that are compatible with translational symmetry elements. With Hermann-Mauguin notation, each position in the symbol specifies a different direction.

www.lightsource.ca Point Groups Table taken from: Sands, D.E., Introduction to Crystallography. (Dover: New York, 1993)

www.lightsource.ca Point Groups – Hermann-Mauguin Each component of the point group symbol corresponds to a different direction. The position of an m refers to a direction normal to a mirror plane. A component combining a rotation axis and mirror plane (i.e. 4/m or “four over m”) refers to a direction parallel a rotation axis and perpendicular the mirror plane. Orthorhombic groups: The three components refer to the three mutually perpendicular crystal axes (x, y, z).

www.lightsource.ca Point Groups – Hermann-Mauguin Tetragonal point groups: The 4-fold axis is parallel the z direction. The second component refers to the equivalent x and y directions, and the third component refers to directions in the xy plane bisecting the x and y axes. Hexagonal and Trigonal point groups: The second component refers to equivalent directions in the plane normal to the main 6-fold or 3-fold axis. Cubic point groups: The first component refers to the cube axes, the second component (3) refers to the four 3-fold axes along the body diagonals, the third component refers to the face diagonals.

www.lightsource.ca Crystal Systems SystemLattice Parameter Restrictions Bravais Lattices Minimum Symmetry Elements Triclinic (Anorthic) a, b, c, α, β, γaPNone Monoclinica, b, c, 90, β, 90mP, mCOne 2-fold axis Orthorhombica, b, c, 90, 90, 90oP, oC, oI, oFThree perpendicular 2-fold axes Trigonala, a, a, α, α, α a, a, c, 90, 90, 120 R hP One 3-fold axis Hexagonala, a, c, 90, 90, 120hPOne 6-fold axis Tetragonala, a, c, 90, 90, 90tP, tIOne 4-fold axis Cubica, a, a, 90, 90, 90 cP, cI, cFFour 3-fold axes

www.lightsource.ca Trigonal System The trigonal system has two distinct types of lattices: 1. A primitive cell can be chosen with a = b, α = β = 90°, γ = 120°. This type is identical to the hexagonal lattice except the trigonal cell has a 3-fold rather than a 6-fold axis. 2. A primitive cell can be chosen with a = b = c, α = β = γ ≠ 90°, this lattice type is called rhombohedral (R). Figure taken from: Sands, D.E., Introduction to Crystallography. (Dover: New York, 1993)

www.lightsource.ca Hexagonal and Rhombohedral Lattices

www.lightsource.ca Point Groups & Space Groups The 32 point groups cover all the possible point symmetry elements which occur in finite molecules To fully describe the symmetry of crystal structures, we need to include two symmetry elements which combine rotation and reflection with the translational symmetry of the lattice (called screw axes and glide planes respectively). Groups which include both the point symmetry elements of finite molecules and the translational elements of a crystal are called space groups.

www.lightsource.ca Screw Axes A screw axis, referred to with the symbol n p, combines two operations; a rotation of 360°/n followed by a translation of p/n in the direction of the axis. Figures taken from: Sands, D.E., Introduction to Crystallography. (Dover: New York, 1993)

www.lightsource.ca Glide Planes A glide plane combines two operations, reflection in a plane followed by translation parallel the plane. A glide parallel the b-axis would be referred to with the symbol b, and consist of a reflection followed by a translation of b/2.

www.lightsource.ca Space Groups By combining the point groups, Bravais lattices and translation symmetry elements (screw axes and glide planes), 230 unique space groups are obtained. Many space groups have multiple settings (and/or choices of origin based on the site symmetry chosen for the origin): Space group number 62 (orthorhombic) Standard setting: Pnma Alternate settings: Pnam, Pmcn, Pcmn, Pbnm, Pmnb Two useful websites for space group information: http://img.chem.ucl.ac.uk/sgp/mainmenu.htm http://www.cryst.ehu.es/

www.lightsource.ca Equivalent Positions The symmetry operations associated with a space group can be used to generate positions which are symmetrically equivalent. Consider tetragonal space group P4/m (#83): For a general point (with coordinates x, y, z), the 4 axis parallel c generates three new points. Each of these four points is then reflected in the z=0 plane (z → -z).

www.lightsource.ca Special Positions (space group P4/m) MultiplicityWyckoffSite SymmetryEquivalent Positions 8l1x, y, z; -y, x, z; -x, -y, z; y, -x, z; x, y, -z; -y, x, -z; -x, -y, -z; y, -x, -z 4kmx, y, ½ ; -y, x, ½; -x, -y, ½; y, -x, ½ 4jmx, y, 0; -y, x, 0; -x, -y, 0; y, -x, 0 4i20, ½, z; ½, 0, z; 0, ½, -z; ½, 0, -z 2h4½, ½, z; ½, ½, -z 2g40, 0, z; 0, 0, -z 2f2/m0, ½, ½; ½, 0, ½ 2e2/m0, ½, 0; ½, 0, 0 1d4/m½, ½, ½ 1c4/m½, ½, 0 1b4/m0, 0, ½ 1a4/m0, 0, 0

www.lightsource.ca Example Structures - Perovskite

www.lightsource.ca Powder Patterns - Perovskite For more details on this system, see: Ali, R. & Yashima, M. J. Solid State Chem. 178 (2005) 2867-2872.

www.lightsource.ca Miller Indices and Interplanar Spacing Crystallographic planes are described using Miller indices (hkl), which are derived from the intercepts of the plane with the crystal axes. Figure courtesy of Michael Gharghouri.

www.lightsource.ca Families of Planes Figure courtesy of Michael Gharghouri.

www.lightsource.ca Systematic Absences

www.lightsource.ca Diffraction - Bragg’s Law

www.lightsource.ca Diffraction Geometry Figure courtesy of Michael Gharghouri.

www.lightsource.ca Single Crystal versus Powder Patterns Debye-Scherrer Cones Powder Single Crystal

www.lightsource.ca Powder Diffraction Geometry Figure taken from: Cockcroft, J.K..& Fitch, A.N. in Powder Diffraction, Theory and Practice. Edited by R.E. Dinnebier & S.J.L. Billinge. (RSC Publishing: Cambridge, 2008) Bragg-Brentano Debye-Scherrer

www.lightsource.ca Reflection Positions - Bragg’s law

www.lightsource.ca Reflection Positions – Systematic Errors

www.lightsource.ca Diffraction Pattern Intensity Structure Factor Multiplicity Factor Texture/ Preferred Orientation Reflection Profile Function Scale Factor (phase p) Absorption Background Lorentz-polarization correction

www.lightsource.ca Scale Factor The scale factor (S p ) is proportional to the quantity of the phase present in the mixture, and can be used to estimate the crystalline phase composition, W p (weight fraction):

www.lightsource.ca Structure Factor Atomic Scattering Factor Thermal (Debye-Waller) Factor Site Occupancy

www.lightsource.ca Atomic Scattering Factor Light elements scatter X- rays relatively poorly. The intensities of X-ray diffraction peaks decrease rapidly with increasing diffraction angle (2θ). Figure taken from: Waseda, Y. et al., X-ray Diffraction Crystallography. (Springer: Berlin, 2011)

www.lightsource.ca Thermal Parameter The thermal parameter reflects thermal motion in the atoms from their equilibrium positions which attenuates the reflection intensities:

www.lightsource.ca Multiplicity Factor The multiplicity reflects the number of equivalent planes (or equivalent grain orientations to diffract) belonging to a set of hkl indices. Systemhklhhlhh00kkhhhhk0h0l0klh00k0000l Cubic48*2412 824* 666 Tetragonal16*84888*88442 Hexagonal24*12*612 12* 662 Orthorhombic88888444222 Monoclinic44444424222 Triclinic22222222222 Figure courtesy of Michael Gharghouri. Asterisk (*) indicates non-equivalence of planes may reduce this number by half in some circumstances.

www.lightsource.ca Further Reading Sands, D.E. Introduction to Crystallography. Dover: New York, 1993. Sands, D.E. Vectors and Tensors in Crystallography. Dover: New York, 2002. Pecharsky, V.K. & Zavalij, P.Y. Fundamentals of Powder Diffraction and Structural Characterization of Materials, 2 nd Ed. Springer: New York, 2009. Warren, B.E. X-ray Diffraction. Dover: New York, 1990. Klug, H.P. & Alexander, L.E. X-ray Diffraction Procedures for Polycrystalline and Amorphous Materials, 2 nd Ed. Wiley: New York: 1974. Young, R.A., ed. The Rietveld Method. Oxford: New York, 1993.

www.lightsource.ca Acknowledgments Much thanks to Michael Gharghouri (NRC Canadian Neutron Beam Centre, Chalk River) and Dover Publications, Inc. for their generous permission to use multiple figure. Thank you to Ian Swainson (Canadian Centre for Nuclear Innovation) and Pawel Grochulski (Canadian Light Source) for helpful suggestions which improved this presentation.

www.lightsource.ca Absorption (Geometry)

www.lightsource.ca Absorption (Geometry) APS beamline 11-BM absorption guide & calculator: http://11bm.xor.aps.anl.gov/absorption.html

www.lightsource.ca Reflection Profile Functions Figure taken from: Kaduk, J.A. & Reid, J. Powder Diffraction 26 (2011) 88-93.

www.lightsource.ca Reflection Profile Functions